Effect of Ultra-Fast Heat Treatment on the Subsequent Formation · PDF file metals Article...
Embed Size (px)
Transcript of Effect of Ultra-Fast Heat Treatment on the Subsequent Formation · PDF file metals Article...
Delft University of Technology
Effect of ultra-fast heat treatment on the subsequent formation of mixed martensitic/bainitic microstructure with carbides in a crmo medium carbon steel
Papaefthymiou, Spyros; Banis, Alexandros; Bouzouni, Marianthi; Petrov, Roumen H.
DOI 10.3390/met9030312 Publication date 2019 Document Version Final published version Published in Metals
Citation (APA) Papaefthymiou, S., Banis, A., Bouzouni, M., & Petrov, R. H. (2019). Effect of ultra-fast heat treatment on the subsequent formation of mixed martensitic/bainitic microstructure with carbides in a crmo medium carbon steel. Metals, 9(3), . https://doi.org/10.3390/met9030312
Important note To cite this publication, please use the final published version (if applicable). Please check the document version above.
Copyright Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons.
Takedown policy Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.
This work is downloaded from Delft University of Technology. For technical reasons the number of authors shown on this cover page is limited to a maximum of 10.
Effect of Ultra-Fast Heat Treatment on the Subsequent Formation of Mixed Martensitic/Bainitic Microstructure with Carbides in a CrMo Medium Carbon Steel
Spyros Papaefthymiou 1,* , Alexandros Banis 1, Marianthi Bouzouni 1,2 and Roumen H. Petrov 3,4
1 Laboratory of Physical Metallurgy, Division of Metallurgy and Materials, School of Mining & Metallurgical Engineering, National Technical University of Athens, 9, Her. Polytechniou str., Zografos, 15780 Athens, Greece; email@example.com (A.B.); firstname.lastname@example.org (M.B.)
2 Department of Physical Metallurgy and Forming, Hellenic Research Centre for Metals S.A.—ELKEME S.A., 61st km Athens-Lamia Nat. Road, 32011 Oinofyta, Viotia, Greece
3 Department of Electrical Energy, Metals, Mechanical constructions & Systems, Ghent University, Technologiepark 46, 9052 Ghent, Belgium; email@example.com
4 Department of Materials Science and Engineering, Delft University of Technology, Mekelweg 2, 2628CD Delft, The Netherlands
* Correspondence: firstname.lastname@example.org; Tel.: +30-210-772-4710
Received: 5 February 2019; Accepted: 4 March 2019; Published: 10 March 2019 ���������� �������
Abstract: The current work focuses on complex multiphase microstructures gained in CrMo medium carbon steel after ultra-fast heat treatment, consisting of heating with heating rate of 300 ◦C/s, 2 s soaking at peak temperature and subsequent quenching. In order to better understand the microstructure evolution and the phenomena that take place during rapid heating, an ultra-fast heated sample was analyzed and compared with a conventionally treated sample with a heating rate of 10 ◦C/s and 360 s soaking. The initial microstructure of both samples consisted of ferrite and spheroidized cementite. The conventional heat treatment results in a fully martensitic microstructure as expected. On the other hand, the ultra-fast heated sample shows significant heterogeneity in the final microstructure. This is a result of insufficient time for cementite dissolution, carbon diffusion and chemical composition homogenization at the austenitization temperature. Its final microstructure consists of undissolved spheroidized cementite, nano-carbides and martensite laths in a ferritic matrix. Based on EBSD and TEM analysis, traces of bainitic ferrite are indicated. The grains and laths sizes observed offer proof that a diffusionless, massive transformation takes place for the austenite formation and growth instead of a diffusion-controlled transformation that occurs on a conventional heat treatment.
Keywords: ultra-fast heating; martensite/bainite; diffusionless transformations; AHSS
Over the last years the research focus was on both strength and toughness increase of advanced high strength steels (AHSS). This was achieved either by introducing multiphase microstructures embedding bainitic ferrite, retained austenite and/or martensite in a ferritic matrix (dual phase—DP, TRansformation Induced Plasticity—TRIP, complex phase—CP steels to name a few), or by getting use of the twinning effect of austenite (Twinning Induced Plasticity—TWIP steels), or by using alloying elements (Mn and AlMn steels) or currently by developing steels with submicron (nano-scaled) mixed grain structure including tempered martensite, retained austenite and bainite (e.g., quenching
Metals 2019, 9, 312; doi:10.3390/met9030312 www.mdpi.com/journal/metals
http://www.mdpi.com/journal/metals http://www.mdpi.com https://orcid.org/0000-0001-8137-938X https://orcid.org/0000-0003-0551-9058 http://www.mdpi.com/2075-4701/9/3/312?type=check_update&version=1 http://dx.doi.org/10.3390/met9030312 http://www.mdpi.com/journal/metals
Metals 2019, 9, 312 2 of 14
& partitioning—Q&P steels) [1–3]. In all these developments attention was given to the chemical composition and the tailored made heat treatment cycles, many of which are achieved in two or more stages. Till now, the effect of increased heating rate during the final heat treatment was not incorporated in the steel development strategies. Fast and ultra-fast heating rates are usually obtained by induction heating combined with a subsequent water or oil quenching. Although there is no clear specification what the borders between normal, fast and ultra-fast heating rates in the existing literature are, the following can be considered: Low and normal heating rates are between 1 ◦C/s and 20 ◦C/s, high heating rates are between 20 ◦C/s and 100 ◦C/s and ultra-fast heating rates are these above 100 ◦C/s. As induction heating is currently introduced as part of the forming process chain (press hardened and air hardened steels) replacing classical gas furnaces, the effect of rapid heating in the ferrite-to-austenite transformations and the carbide dissolution must gain more attention [4–7]. At increasing heating rates above 100 ◦C/s the resulting microstructures differ from those after conventional heat treatments [4,5,8,9]. The reason is that the ferrite to austenite phase transformation during ultra-fast heating creates chemically and structurally (morphologically) heterogeneous austenite with very fine grains which transforms after quenching to mixtures of bainite & martensite and finely dispersed carbides . The latter in combination with the dislocation density introduced during displacive transformations will further impede the final thickness of martensitic or bainitic plates and sheaves respectively [11–13]. Moreover, the presence of substitutional atoms e.g., Cr and Mn, which tend to segregate at interfaces can modify the local equilibrium and affect the subsequent phase transformations [14–18]. Other alloying elements such as Si suppress the carbide precipitation during the bainitic transformation and stimulate the retention of austenite at room temperature. The above mechanisms may lead to formation of multiphase microstructures consisting of martensitic, bainitic ferritic plates with high and low carbon content often accompanied with M–A (martensite–austenite) islands .
With the recent developments in microstructure and crystallographic analysis (scanning and transmission electron microscopy SEM & TEM—STEM, electron backscatter diffraction EBSD, transmission Kikuchi diffraction—TKD) it is possible to distinguish and quantify these nano—constituents in order to understand the mechanism of their formation and their impact on the mechanical properties .
The ultra-fast heat treatment e.g., via induction heating utilizes the effect of the rapid heating to restrict the austenite grain size and its chemical composition prior to quenching. In this way, a mixed martensite/bainite microstructure matrix with embedded carbides can be obtained in one step paving the way for increased and more isotropic mechanical properties of the treated steel. The ultra-fast heat treatment was introduced in sheets and tubes by Cola et al. [21–24] in which a large variety of refined microstructures and properties were derived. The ultra-fast heat treatment in steels affects the microstructure additionally by creating a conditions ferrite -to–austenite phase transformation to start and progress in non-recrystallized or partially recrystallized (recovered) matrix which reflects in better mechanical properties, namely increase of both strength and elongation [25–27]. The impact of heating rate on phase composition and volume fraction of individual micro-constituents has been studied as well . Ultra-fast heating of a low-carbon steel to inter-critical peak temperature prompts to a complex microstructure of the ferritic matrix, which comprises of recrystallized and recovered grains [29–31]. Thus, the local mechanical behavior of the ferritic matrix may drastically vary upon the local dislocation density.
Cerda et al. [32,33] studied the effect of ultra-fast heating on the recrystallization of ferrite. In another study the same authors [34–36] explained the impact of the initial microstructure on the austenite formation mechanism and that the nucleation step can be obtained either by diffusion or diffusionless mechanisms, while th